advertisement

PHYSICAL REVIEW B 73, 014512 共2006兲 Dendritic and uniform flux jumps in superconducting films D. V. Denisov,1,2 A. L. Rakhmanov,3 D. V. Shantsev,1,2 Y. M. Galperin,1,2,4 and T. H. Johansen1,* 1Department of Physics and Center for Advanced Materials and Nanotechnology, University of Oslo, P.O. Box 1048 Blindern, 0316 Oslo, Norway 2 A. F. Ioffe Physico-Technical Institute, Polytekhnicheskaya 26, St. Petersburg 194021, Russia 3Institute for Theoretical and Applied Electrodynamics, Izhorskaya 13/19, Moscow 125412, Russia 4Argonne National Laboratory, 9700 South Cass Avenue, Argonne, Illinois 60439, USA 共Received 7 October 2005; published 13 January 2006; publisher error corrected 15 February 2006兲 Recent theoretical analysis of spatially-nonuniform modes of the thermomagnetic instability in superconductors 关Phys. Rev. B 70, 224502 共2004兲兴 is generalized to the case of a thin film in a perpendicular applied field. We solve the thermal diffusion and Maxwell equations taking into account nonlocal electrodynamics in the film and its thermal coupling to the substrate. The instability is found to develop in a nonuniform, fingering pattern if the background electric field, E, is high and the heat transfer coefficient to the substrate, h0, is small. Otherwise, the instability develops in a uniform manner. We find the threshold magnetic field, Hfing共E , h0兲, the characteristic finger width, and the instability buildup time. Thin films are found to be much more unstable than bulk superconductors, and have a stronger tendency for formation of fingering 共dendritic兲 pattern. DOI: 10.1103/PhysRevB.73.014512 PACS number共s兲: 74.25.Qt, 74.25.Ha, 68.60.Dv I. INTRODUCTION II. MODEL AND BASIC EQUATIONS The thermomagnetic instability or flux jumping is commonly observed at low temperatures in type-II superconductors with strong pinning.1–4 The instability arises for two fundamental reasons: 共i兲 motion of magnetic flux releases energy, and hence increases the local temperature; 共ii兲 the temperature rise decreases flux pinning, and hence facilitates the further flux motion. This positive feedback can result in thermal runaways and global flux redistributions jeopardizing superconducting devices. The conventional theory of the thermomagnetic instability1,2 considers only “uniform” flux jumps, where the flux front is smooth and essentially straight. This picture is true for many experimental conditions, however, far from all. Numerous magneto-optical studies have recently revealed that the thermomagnetic instability in superconductors can result in strongly branched dendritic flux patterns.5–19 In a recent paper we examined the problem of flux pattern formation in the slab geometry.20 Experimentally, however, the dendritic flux patterns are mostly observed in thin film superconductors placed in a perpendicular magnetic field. An analysis of this perpendicular geometry was recently published by Aranson et al.21 Here we present a more exact and complete picture of the dendritic instability and analyze the criteria of its realization. In the following we restrict ourselves to a conventional linear analysis1,2,22 of the instability and consider the spacetime development of small perturbations in the electric field, E, and temperature, T. In contrast to the slab case,20 the heat transfer from the superconductor to a substrate as well as the nonlocal electrodynamics in thin films are taken into account. Consequently, the results depend significantly on the heat transfer rate, h0, as well as on the film thickness, d. Our main result is that the instability in the form of narrow fingers perpendicular to the background field, E, occurs much easier in thin films than in slabs and bulk samples, and the corresponding threshold field, Ec, is found to be proportional to the film thickness, d. Consider the perpendicular geometry shown in Fig. 1, with a thin superconducting strip placed in a transverse magnetic field, H. The strip is infinite along the y axis, and occupies the space from −d / 2 to d / 2 in the z direction and from 0 to 2w in the x direction. It is assumed that d Ⰶ w. In the unperturbed state the screening current flows along the y axis. The distributions of the current density, j, and magnetic induction, B, in the flux penetrated region 0 ⬍ x ⬍ ᐉ are determined by the Maxwell equation 1098-0121/2006/73共1兲/014512共7兲/$23.00 curl B = 0j, 共1兲 where the common approximation B = 0H is used. To find the electric field and the temperature we use another Maxwell equation together with the equation for thermal diffusion curl E = − B/t, 共2兲 FIG. 1. 共Color online兲 A superconductor strip on a substrate 共only the left half is shown兲. The dark gray area is the fluxpenetrated region. 014512-1 ©2006 The American Physical Society PHYSICAL REVIEW B 73, 014512 共2006兲 DENISOV et al. C共T/t兲 = ⵜ2T + jE. 共3兲 Here C and are the specific heat and thermal conductivity, respectively. Equations 共1兲–共3兲 should be supplemented by a currentvoltage relation j = j共E , B , T兲. For simplicity we assume a current-voltage curve of the form j = jc共T兲g共E兲共E/E兲. 共4兲 Whereas it follows from symmetry considerations that Ex = 0, both components of the perturbation, ␦E, will in general not vanish. Linearizing the current-voltage relation, Eq. 共4兲 one obtains ␦j = 共5兲 Here is the differential electrical conductivity, 共E兲 ⬅ j / E. The parameter n generalizes the exponent in the frequently used power-law relation E ⬀ jn with n independent of E. The key dimensionless parameter of the model is the ratio of thermal and magnetic diffusion coefficients,1 ⬅ 0/C. 共6兲 The smaller is, the slower heat diffuses from the perturbation region into the surrounding areas. Hence, one can expect that for smaller : 共i兲 the superconductor is more unstable, and 共ii兲 the formation of instability-induced nonuniform structures is more favorable. In the following we assume that the strip is thinner than the London penetration depth, L, and at the same time much wider than the effective penetration length, eff = L2 / d 共8兲 ␦T = T* exp共t/t0 + ikx + iky兲, ␦Ex,y = Ex,y exp共t/t0 + ikx + iky兲, ␦ jx,y = jcix,y exp共t/t0 + ikx + iky兲, 共9兲 where , , and i are z-dependent dimensionless Fourier amplitudes. The coordinates are normalized to the adiabatic length a = 冑CT* / 0 j2c where T* = −共 ln jc / T兲−1 is the characteristic scale of the temperature dependence of jc, so that = x / a, = y / a, = z / a. The time is normalized to t0 = CT* / j2c = 0a2, which is the magnetic diffusion time for the length a. Re is the dimensionless instability increment, which when positive indicates exponential growth of the perturbation. We can now use the formulas 共9兲 to rewrite the basic equations in dimensionless variables. From Eq. 共8兲 one finds for the components of the current density perturbation i i x = x, iy = − + n−1y . 共10兲 Combining the Maxwell equations 共1兲 and 共2兲, and the thermal diffusion equation 共3兲 yields k ⫻ 关k ⫻ 兴 = ni, d 艋 L Ⰶ 冑dw. The stationary current and field distributions in a thin strip under such conditions were calculated by several authors,24–26 finding that the flux penetration depth, ᐉ, is related to the applied field by the expression 冊 ␦Ex jc E . + jc ␦T + ␦E y E T E We shall seek perturbations in the form A strong nonlinearity of the function g共E兲 leads to formation of a quasistatic critical state with j ⬇ jc共T兲, where jc is the critical current density.23 We neglect any B dependence of jc, i.e., adopt the Bean model. The exact form of g共E兲 is not crucially important, the only issue is that it represents a very steep E共j兲 curve having a large logarithmic derivative n共E兲 ⬅ ln E/ ln j ⬇ jc/E Ⰷ 1. 冉 冉 = − k2y + 共11兲 冊 2 + 共iy + y兲/n. 2 共12兲 Here it is assumed that the penetration is shallow, or more precisely that eff Ⰶ ᐉ Ⰶ w. Magneto-optical imaging shows that flux patterns produced by the dendritic instability5–19 are characterized by having ky Ⰷ kx. Therefore, we have neglected the heat flow along the x direction compared to that along the y direction. Later we will check the consistency of this assumption by showing that indeed the fastest growing perturbation has ky Ⰷ kx. III. PERTURBATION ANALYSIS B. Boundary conditions ᐉ/w = 2H2/2d2 j2c . 共7兲 A. Linearized dimensionless equations We seek solutions of Eqs. 共1兲–共4兲 in the form T + ␦T共x,y,z,t兲, E + ␦E共x,y,z,t兲, j + ␦j共x,y,z,t兲, where T, E, and j are background values. The background electric field may be created, e.g., by ramping the external magnetic field, and for simplicity we assume it to be coordinate independent. Allowing for such a dependence would only lead to insignificant numerical corrections, as discussed in Ref. 20. Similarly, we will assume a uniform background temperature. We assume that heat exchange between the superconducting film and its environment follows the Newton cooling law. For simplicity we let the boundary condition, ⵜ 共T + ␦T兲 = −h0共T + ␦T − T0兲, apply to both film surfaces. Here T0 and h0 are the effective environment temperature and heat transfer coefficient, respectively. Equations 共12兲 and 共10兲 can now be integrated over the film thickness to yield = where 014512-2 共1 + n−1兲y n + n共k2y + h兲 + 1 , PHYSICAL REVIEW B 73, 014512 共2006兲 DENDRITIC AND UNIFORM FLUX JUMPS IN¼ h = 2h0a2/d. In the remaining part of the paper we let , , and i denote perturbations averaged over the film thickness. We seek a solution of the electrodynamic equations in the flux penetrated region, 0 艋 艋 ᐉ / a. At the film edge, = 0, one has ␦ jx = 0 and, consequently, ␦Ex = 0. In the Meissner state both the electric field and heat dissipation are absent, so that ␦Ey = ␦T = ␦ j y = 0 at the flux front, = ᐉ / a. Thus, the Fourier expansions for the x and y components of electric field perturbation will contain only sin共kx兲 and cos共kx兲, respectively. Then the boundary conditions are satisfied for kx = 共a/2ᐉ兲共2s + 1兲, s = 0,1,2, . . . . Since ᐉ depends on the magnetic field, the values of kx are also magnetic field dependent. Now we can integrate Eq. 共11兲 over the film thickness and employ the symmetry of the electrodynamic problem with respect to the plane z = 0. It yields − iky共kxy + ikyx兲 − ␦E⬘x,y/E = ⫿ n␦By,x/0ajc . 共13兲 Due to continuity of the magnetic field tangential components Eq. 共15兲 is also valid at the film surface, = d / 2a. Thus it can be substituted into Eqs. 共14兲. The Fourier components of the kernel function G共 , 兲 with respect to can be calculated directly yielding G共,ky兲 = kya K1关ky冑2 + 共d/2a兲2兴 , 2ᐉ 冑2 + 共d/2a兲2 − ikxkyy + 共k2y + n兲x = 共d/2a兲n 兺 Gx共kx,kx⬘,ky兲x共kx⬘兲, kx⬘ 共17兲 共14兲 共k2x + nf兲y + ikxkyx = 共d/2a兲nf 兺 Gy共kx,kx⬘,ky兲y共kx⬘兲, kx⬘ We have here introduced the function f共,ky兲 ⬅ 1 + n−1 iy 1 − . y n n + n共k2y + h兲 + 1 再 Note that the equation for the z component of the field is satisfied automatically. The derivatives ⬘x,y with respect to are taken at the film surface, = d / 2a. To calculate them, one needs the electric field distribution outside the superconductor, where the flux density is given by the Bio-Savart law B共r兲 = 0H + 0 4 冕 d 3r ⬘ 冕 ⬘冕 ᐉ/a 0 G共, 兲 = d ⬁ Gy共kx,kx⬘,ky兲 冎 冕 冕 ᐉ/a =4 再 d d⬘G共 − ⬘,ky兲 0 0 ⫻ ᐉ/a sin共kx兲sin共kx⬘⬘兲 cos共kx兲cos共kx⬘⬘兲 冎 . ␣ = d/2ᐉ Ⰶ 1. 共19兲 共20兲 One can then find analytical expressions for the kernel, and it turns out that only its diagonal part, kx = kx⬘, is important. In this paper we present analytical expressions up to the first order in ␣, while the plots are calculated up to the second order. The second-order analytical expressions can be found in Ref. 27. The kernel 共19兲 can be written as d⬘G共 − ⬘, − ⬘兲␦ j y,x , −⬁ 1 . 4关 + + 共d/2a兲2兴3/2 2 Gx共kx,kx⬘,ky兲 共18兲 We are interested only in the specific case of a very thin strip j ⫻ 共r − r⬘兲 . 兩r − r⬘兩3 The perturbation of flux density is then ␦Bx,y = ± 0d 共16兲 where K1 is the modified Bessel function of the second kind. The above Fourier expansions in cos共kx兲 and sin共kx兲 correspond to the finite interval −2ᐉ / a ⬍ ⬍ 2ᐉ / a. Therefore we should continue x,y from 0 ⬍ ⬍ ᐉ / a to this interval and then introduce Gx and Gy as analytical continuations of G共 − ⬘ , ky兲 having the same symmetry as x and y, respectively 共see Ref. 27 for details兲. All this allows us to rewrite the set 共14兲 as 2a ⬘ = − nx , d x 2a − kx共kxy + ikyx兲 + ⬘y = − nf共,ky兲y . d 共15兲 2 Gx,y共kx,kx,ky兲 = Here we have approximated the average over ⬘ substituting ⬘ = 0. In this way we omit only terms of the order of 共d / a兲2 Ⰶ 1. The integration over ⬘ should, in principle, cover also the Meissner region, ⬘ ⬎ l / a. Though the flux density there remains zero during the development of perturbation, the Meissner current will be perturbed due to the nonlocal current-field relation. However the kernel G共 , 兲 decays very fast at distances larger than d / a and therefore the Meissner current perturbation produces only insignificant numerical corrections. The perturbation of the magnetic field can be related to that of the electrical field by Eq. 共2兲, which can be rewritten as 冋 册 a 1 − ␥共␣,kx兲␣ , ᐉ ␣ 共21兲 where ␥共␣ , kx兲 is a dimensionless function. In what follows we shall consider only the main instability mode, kx = a / 2ᐉ, which turns out always to be the most unstable one. For this mode, and in the limit ␣ → 0, the function ␥共␣ , kx兲 approaches a constant value ⬇5. Substituting the above expression for G into Eqs. 共17兲 and 共18兲 one obtains the dispersion relation for 共kx , ky兲 A12 + A2 + A3 = 0. Here 014512-3 A1 = n␥␣, A2 = k2y 共1 + A1兲 + nk2x + A1共h − 1兲, 共22兲 PHYSICAL REVIEW B 73, 014512 共2006兲 DENISOV et al. as H ⬎ Hadiab, with the adiabatic instability field Hadiab = FIG. 2. 共Color online兲 The solutions of dispersion equation 共22兲 for small and large , for ␣ = 0.001 and n = 20. = − 共k2y + h兲 + 冑 d slab H . w adiab 共24兲 共k2y − k2x 兲 k2y + nk2x . From this expression we obtain IV. RESULTS k*x = 共冑n + 1 − 冑nh兲/n冑 , Let us first consider the simple case of a uniform perturbation, ky = 0. One finds from Eq. 共22兲 that the perturbation will grow 共Re ⬎ 0兲 if h ⬍ 1 − d CT* ⬃ w ␥0 slab is the adiabatic instability field for the slab Here Hadiab geometry.1–4,22 This result coincides up to a numerical factor with the adiabatic instability field for a thin strip found recently in Ref. 28. Solutions of Eq. 共22兲 for perturbations with arbitrary ky are presented in Fig. 2. The upper panel shows Re 共ky兲 curves for = 0.01 and different values of kx. For large kx, i.e., small magnetic field, Re is negative for all ky. It means that the superconductor is stable. However, at small kx, the increment Re becomes positive in some finite range of ky. Hence, some perturbations with a spatial structure will start growing. They will have the form of fingers of elevated T and E directed perpendicularly to the flux front. We will call this situation the fingering (or dendritic) instability. For large an instability also develops at small kx, however in a different manner, see Fig. 2 共lower panel兲. Here the maximal Re always corresponds to ky = 0. Hence, the uniform perturbation will be dominant. The uniform growth of perturbations for large has been recently predicted in Refs. 20 and 21 and explained by the prevailing role of heat diffusion. Let us now find the critical k*y and k*x for the fingering instability, see Fig. 2 共upper panel兲. The k*x determines the applied magnetic field when the instability first takes place, while k*y determines its spatial scale. These quantities can be found from the requirement max兵Re 共ky兲其 = 0 for ky ⫽ 0. In the limit ␣ Ⰶ 1 we can put A1 = 0 in Eq. 共22兲 and then rewrite it in the form A3 = k4y + nk2x k2y + nk2x 共h + 1/n兲 + k2y 共h − 1兲. k2x /␥␣ . 冑 共23兲 When the flux penetration region, ᐉ, is small, i.e., kx is large, the system is stable. As the flux advances, kx decreases, and the system can eventually become unstable. The instability will take place, however, only if h ⬍ 1. Otherwise the superconducting strip of any width will remain stable no matter how large a magnetic field is applied. This size-independent stability means that at h 艌 1 the heat dissipation due to flux motion is slower than heat removal into the substrate. Equation 共23兲 further simplifies in the adiabatic limit, → 0, when the heat production is much faster than heat diffusion within the film or into the substrate. The instability then develops at k2x / 共␥␣兲 ⬍ 1, which in dimensional variables reads as 0 j2c ld ⬎ CT*共2 / 2␥兲. Assuming small penetration depth, l Ⰶ w, and using Eq. 共7兲 this criterion can be rewritten k*y = 关冑nh + 1共冑n + 1 − 冑nh + 1兲兴1/2/冑n . k*x , k*y 共25兲 on the heat transfer coefficient The dependences of h are shown in Fig. 3. One can see that k*y is always larger than k*x implying that fingers of elevated T and E are extended in the direction normal to the film edge. For h Ⰶ 1 / and n Ⰷ 1 we find k*y ⬇ n1/4k*x Ⰷ k*x ⬇ 1 / 冑n. Both k*x and k*y tend to zero as h → 1 / , while for larger h the system is always stable due to fast heat removal to the substrate. It follows from Fig. 2 that for large enough the instability will develop uniformly, while for small it will acquire a spatially-nonuniform structure. Let us find now the critical value c that separates these two regimes. It can be obtained from the equality Re 共kx = k*x , ky = 0兲 = 0. When it is fulfilled Re = 0 both for ky = 0 and for ky = k*y ⫽ 0. We find using Eq. 共22兲 that the instability will evolve in a spatially nonuniform way if 014512-4 PHYSICAL REVIEW B 73, 014512 共2006兲 DENDRITIC AND UNIFORM FLUX JUMPS IN¼ FIG. 3. Dependences of k*y and k*x on h for n = 20, = 0.01, ␣ = 0.001 according to Eq. 共25兲. ⬍ c = 共1 − k*2 x /␥␣兲/h. 共26兲 Substituting here ␣ and k*x we find a transcendental relation between c and h. For n Ⰷ 1 it reduces to 冑nc共1 + 冑hc兲 = a/␥d. FIG. 5. 共Color online兲 Stability diagram in the H-E plane according to Eqs. 共23兲 and 共25兲. hcrit = 共28兲 and the critical electric field Ec for h0 = 0 is 共27兲 Using this result we can construct a stability diagram in the E-h0 plane shown in Fig. 4. The curved line marks the critical electric field Ec共h0兲 that separates two types of instability: fingering 共E ⬎ Ec兲 and uniform 共E ⬍ Ec兲. This line is calculated from Eq. 共27兲, where the electric field is expressed via as E = jc0 / nC according to Eqs. 共5兲 and 共6兲. The straight line is given by the condition h = 1. Below this line the superconductor is always stable, as follows from Eq. 共23兲 for the uniform perturbations, and from Eq. 共25兲 for the nonuniform case. At a certain value h0 = hcrit, the two lines intercept. We find 2␥220 j4c d3n , 2T*2C2 Ec共0兲 = ␥220 j3c 2 d , 2C 2T * 共29兲 while Ec共hcrit兲 = 4Ec共0兲. For any point 共h0 , E兲 belonging to the stable phase in the stability diagram, Fig. 4, the flux distribution is stable for any applied magnetic field. For the points belonging to unstable phases, the instability develops above some threshold magnetic field, either Hfing共h0 , E兲 or Huni共h0 , E兲 for fingering or uniform instability, respectively. Shown in Fig. 5 are three sets of Hfing共E兲 and Huni共E兲 curves for different values of h0. They represent boundaries between the three phases, stable and unstable with respect to either fingering or uniform instability, as shown in the inset. Using Eq. 共7兲 one can rewrite the expression 共23兲 for Huni as 冉 Huni = Hadiab 1 − 2T*h0 ndjcE 冊 −1/2 . 共30兲 In the absence of heat removal to the substrate, h0 = 0, we obtain the adiabatic instability field, Eq. 共24兲, and the Huni共E兲 curve becomes a horizontal line.29 The threshold magnetic field for the fingering instability, Hfing, is calculated from Eq. 共25兲. A simplified expression obtained for h Ⰶ 1 / and n Ⰷ 1 冉 冑 冊 j cd 2 Hfing = w FIG. 4. 共Color online兲 Stability diagram in the plane electric field, heat transfer coefficient according to Eq. 共27兲, and condition 1 − h ⬎ 0 for n = 30 and ␣ = 0.001. T* j c E 1/2 , 共31兲 shows that at large electric fields Hfing decays as E−1/4. At h0 艋 hcrit the curves Hfing共E兲 and Huni共E兲 intercept at the critical electric field Ec determined by Eq. 共26兲. At h0 艌 hcrit we have Hfing共E兲 ⬍ Huni共E兲 for any E, so the lines do not intercept and the instability will develop into a fingering pattern. 014512-5 PHYSICAL REVIEW B 73, 014512 共2006兲 DENISOV et al. V. DISCUSSION Let us compare the present results for a thin film in a perpendicular magnetic field with results of Ref. 20 for a bulk superconductor. In both cases the instability develops into a fingering pattern if the background electric field in the superconductor exceeds some critical value Ec. The values of Ec are however different. Their ratio for a thin strip and a slab Ec共0兲 Eslab c = ␥2 d2 j2c 0 , 2 CT* 共32兲 is expected to be much less than unity. For jc = 1010 A / m2, C = 103 J / Km3, = 10−2 W / Km, T* = 10 K, and d = 0.3 m, we find from Eq. 共29兲 that Ec ⬇ 4 ⫻ 10−4 V / m, while according to Ref. 20, Eslab c = 0.1 V / m. Consequently, the development of thermomagnetic instability into a fingering pattern is much more probable in thin films than in bulk superconductors. The threshold magnetic field for the fingering instability, Hfing, is also much smaller for thin films. Comparing Eq. 共31兲 with the results of Ref. 20 for a slab20 we find Hfing 冑2 d . slab = 冑wl* Hinst 共33兲 Here l* = 共 / 2兲冑T* / jcE is the flux penetration depth at the threshold of the fingering instability, H = Hfing. Experimentally, the fingering instability always starts after the flux has penetrated a noticeable distance from the edges, such that l* Ⰷ d.5–19 Hence, for a thin film the fingering instability should start at much smaller applied fields than in bulk samples 共by a factor of ⬃103 for films with d ⬃ 10−4w兲. The difference between the threshold fields for the two geometries here is even stronger than for the case of uniform instability in the adiabatic limit, see Eq. 共24兲. Assuming the above values of parameters and w = 2 mm we find from Eq. 共31兲 that Hfing关Ec共0兲兴 = Hadiab ⬇ 1 mT. This value becomes larger if we take into account the heat transfer to the substrate. It is therefore in excellent agreement with the experiment,8–10,13,16,17,19,28 where the threshold field is typically of the order of a few mTesla. The spatial structure of the instability predicted by our linear analysis is a periodic array of fingers perpendicular to the film edge. Its period can be estimated from Eq. 共25兲. For E = Ec, h = 0 and n Ⰷ 1 one finds dy = 2CT* , 2␥n1/40 j2c d 共34兲 which yields dy ⬇ 100 m for n = 30. Numerical analysis of the instability development shows20,21 that beyond the linear regime the periodic structure is destroyed and only one 共strongest兲 finger invades the Meissner region. This scenario is indeed reproduced experimentally, and the observed width of individual fingers, 20– 50 m,6,8,11,13 is very close to our estimate, dy / 2. The finger width and the threshold magnetic field also depend on the dimensionless parameter h characterizing the thermal coupling to the substrate, Eq. 共13兲. In turn, h, grows rapidly with temperature because of a strong T dependence of C and jc. One can therefore make several testable predictions from the dependences k*x 共h兲 and k*y 共h兲 shown in Fig. 3: 共i兲 There must be a threshold temperature Tth above which the instability is not observed. 共ii兲 When approaching Tth, the instability field diverges since k*x → 0. 共iii兲 When approaching Tth the characteristic width of individual fingers increases since k*y → 0. The last prediction has also been obtained in the boundary layer model allowing calculation of the exact finger shape.31 The first and the second predictions have already been confirmed experimentally.9,11 As for the last one, the T dependence of the finger width has not yet been studied. At the same time, there is a solid experimental evidence8,9,11,19 for an enhanced degree of branching as T → Tth that can be quantitatively described as a larger fractal dimension of the flux pattern.19 This abundant branching could be an indirect consequence of the increased finger width since wider fingers are presumably more likely to undergo splitting. The present problem of fingering instability in a thin film has two new features compared to a similar problem for a bulk superconductor, 共i兲 nonlocal electrodynamics and 共ii兲 thermal coupling to the substrate. The nonlocality results in much smaller values of the threshold magnetic field Hfing and the critical electric field Ec in films than in bulks. If a film is made thinner, it becomes even more unstable since Hfing ⬀ d, and has a stronger tendency to form a fingering pattern since Ec共0兲 ⬀ d2. The thermal coupling to the substrate has a somewhat opposite effect. It can lead to an ultimate stability if h ⬎ 1 / , a situation that is never realized in bulks. A moderate coupling, h Ⰶ 1 / , slightly renormalizes Hfing and Ec, i.e., makes the film a little bit more stable and less inclined to fingering. Let us now compare the results presented in this work to those obtained in a similar model by Aranson et al.21 Our expressions for the “fingering” threshold field, Eq. 共31兲, and for the finger width, Eq. 共34兲, agree with their results up to a numerical factor. For Ⰷ 1 our results for the “uniform” threshold field 关derived from Eq. 共23兲兴 are also similar to results of Ref. 21. As a new result, we find that there exists a critical value of the parameter , Eq. 共26兲, which controls whether the instability evolves either in the uniform, or in the fingering way. Shown in Fig. 4 is the stability diagram where the line Ec共h0兲 separates regimes of fingering and uniform instability. Other results of this paper are 共i兲 the existence of a field-independent “critical point,” hcrit, such that for h0 ⬎ hcrit the instability always develops into a fingering pattern, and 共ii兲 the full stability diagram in the H-E plane, Fig. 5, containing all three phases. The background electric field needed to nucleate the fingering instability can be induced by ramping the magnetic field, E ⬃ Ḣl ⬀ ḢH2 for l Ⰶ w, where Ḣ is the ramp rate. This is the lowest estimate since the flux penetration in practice is strongly nonuniform in space and in time,30 and there can be additional sources of E due to random fluctuations of superconducting parameters. The occurrence of the fingering instability even at rather low ramp rates5,8–10,13,16–19 is therefore not surprising. The buildup time of the instability can be estimated as t0 ⬇ 0.1 s if the flux-flow conductivity = 109 ⍀−1 m−1. Our 014512-6 PHYSICAL REVIEW B 73, 014512 共2006兲 DENDRITIC AND UNIFORM FLUX JUMPS IN¼ linear analysis assumes that the perturbations of T and E grow in amplitude, but remain localized within the initial flux penetrated region. Numerical results show20,21 that at t Ⰷ t0 the perturbations also propagate into the Meissner region. This propagation can be described by recent models32,33 that predict a characteristic propagation speed in agreement with experimental values of 10– 100 km/ s.6,7 In conclusion, the linear analysis of thermal diffusion and Maxwell equations shows that a thermomagnetic instability in a superconducting film may result in either uniform or finger-like distributions of T, E, and B. The fingering distributions will be observed if the background electric field E ⬎ Ec, where Ec grows with the film thickness, the critical current density, the thermal conductivity and the thermal *Electronic address: t.h.johansen@fys.uio.no 1 R. G. Mints and A. L. Rakhmanov, Rev. Mod. Phys. 53, 551 共1981兲. 2 A. Vl. Gurevich, R. G. Mints, and A. L. Rakhmanov, The Physics of Composite Superconductors 共Begell House Inc., New York, 1997兲. 3 S. L. Wipf, Cryogenics 31, 936 共1991兲. 4 Martin N. Wilson, Superconducting Magnets 共Clarendon Press, Oxford, 1983兲. 5 M. R. Wertheimer and J. de G. Gilchrist, J. Phys. Chem. Solids 28, 2509 共1967兲. 6 P. Leiderer, J. Boneberg, P. Brull, V. Bujok, and S. Herminghaus, Phys. Rev. Lett. 71, 2646 共1993兲. 7 U. Bolz, B. Biehler, D. Schmidt, B.-U. Runge, and P. Leiderer, Europhys. Lett. 64, 517 共2003兲. 8 C. A. Duran, P. L. Gammel, R. E. Miller, and D. J. Bishop, Phys. Rev. B 52, 75 共1995兲. 9 M. S. Welling, R. J. Westerwaal, W. Lohstroh, and R. J. Wijngaarden, Physica C 411, 11 共2004兲. 10 T. H. Johansen, M. Baziljevich, D. V. Shantsev, P. E. Goa, Y. M. Galperin, W. N. Kang, H. J. Kim, E. M. Choi, M.-S. Kim, and S. I. Lee, Europhys. Lett. 59, 599 共2002兲. 11 T. H. Johansen, M. Baziljevich, D. V. Shantsev, P. E. Goa, Y. M. Galperin, W. N. Kang, H. J. Kim, E. M. Choi, M.-S. Kim, and S. I. Lee, Supercond. Sci. Technol. 14, 726 共2001兲. 12 A. V. Bobyl, D. V. Shantsev, T. H. Johansen, W. N. Kang, H. J. Kim, E. M. Choi, and S. I. Lee, Appl. Phys. Lett. 80, 4588 共2002兲. 13 F. L. Barkov, D. V. Shantsev, T. H. Johansen, P. E. Goa, W. N. Kang, H. J. Kim, E. M. Choi, and S. I. Lee, Phys. Rev. B 67, 064513 共2003兲. 14 D. V. Shantsev, P. E. Goa, F. L. Barkov, T. H. Johansen, W. N. Kang, and S. I. Lee, Supercond. Sci. Technol. 16, 566 共2003兲. 15 Zuxin Ye, Qiang Li, G. D. Gu, J. J. Tu, W. N. Kang, Eun-Mi Choi, Hyeong-Jin Kim, and Sung-Ik Lee, IEEE Trans. Appl. Supercond. 13, 3722 共2003兲. 16 I. A. Rudnev, S. V. Antonenko, D. V. Shantsev, T. H. Johansen, coupling to the substrate. Due to nonlocal electrodynamics in thin films they turn out to be more unstable than bulk superconductors and more susceptible to formation of a fingering pattern. ACKNOWLEDGMENTS This work is supported by the Norwegian Research Council, Grant No. 158518/431 共NANOMAT兲, by the U. S. Department of Energy Office of Science through Contract No. W-31-109-ENG-38 and by the Russian Foundation for Basic Research through Project No. 03-02-16626. We are thankful for helpful discussions with V. Vinokur, A. Gurevich, I. Aranson, U. Welp, R. Wijngaarden, and V. Vlasko-Vlasov. and A. E. Primenko, Cryogenics 43, 663 共2003兲. C. Wimbush, B. Holzapfel, and Ch. Jooss, J. Appl. Phys. 96, 3589 共2004兲. 18 M. Menghini, R. J. Wijngaarden, A. V. Silhanek, S. Raedts, and V. V. Moshchalkov, Phys. Rev. B 71, 104506 共2005兲. 19 I. A. Rudnev, D. V. Shantsev, T. H. Johansen, and A. E. Primenko, Appl. Phys. Lett. 87, 042502 共2005兲. 20 A. L. Rakhmanov, D. V. Shantsev, Y. M. Galperin, and T. H. Johansen, Phys. Rev. B 70, 224502 共2004兲. 21 I. S. Aranson, A. Gurevich, M. S. Welling, R. J. Wijngaarden, V. K. Vlasko-Vlasov, V. M. Vinokur, and U. Welp, Phys. Rev. Lett. 94, 037002 共2005兲. 22 S. L. Wipf, Phys. Rev. 161, 404 共1967兲. 23 C. P. Bean, Rev. Mod. Phys. 36, 31 共1964兲. 24 E. Zeldov, J. R. Clem, M. McElfresh, and M. Darwin, Phys. Rev. B 49, 9802 共1994兲. 25 E. H. Brandt and M. Indenbom, Phys. Rev. B 48, 12893 共1993兲. 26 W. T. Norris, J. Phys. D 3, 489 共1970兲. 27 A. L. Rakhmanov, D. V. Denisov, D. V. Shantsev, Y. M. Galperin, and T. H. Johansen, cond-mat/0508679 共2005兲. 28 D. V. Shantsev, A. V. Bobyl, Y. M. Galperin, T. H. Johansen, and S. I. Lee, Phys. Rev. B 72, 024541 共2005兲. 29 Strictly speaking Huni should increase at very small E the same way it does in bulk superconductors 共Refs. 1 and 20兲. This behavior is not reproduced in our model since we neglected the heat flow in the x direction. This flow becomes important only in the limiting case h0 → 0. In practice, the heat removal from a thin film to the substrate usually dominates the lateral heat diffusion in the film. 30 E. Altshuler and T. H. Johansen, Rev. Mod. Phys. 76, 471 共2004兲. 31 C. Baggio, R. E. Goldstein, A. I. Pesci, and W. van Saarloos, Phys. Rev. B 72, 060503共R兲 共2005兲. 32 B. Biehler, B.-U. Runge, P. Leiderer, and R. G. Mints, Phys. Rev. B 72, 024532 共2005兲. 33 B. Rosenstein, B. Ya. Shapiro, and I. Shapiro, Europhys. Lett. 70, 506 共2005兲. 17 S. 014512-7